| ||Format||Pages||Price|| |
|11||$60.00||  ADD TO CART|
|Hardcopy (shipping and handling)||11||$60.00||  ADD TO CART|
Significance and Use
6.1 This test method is useful for research and development, quality assurance, regulatory compliance and specification-based acceptance.
6.2 The kinetic parameters determined by this method may be used to calculate thermal hazard figures-of-merit according to Practice .
1.1 This test method describes the determination of the kinetic parameters of Arrhenius activation energy and pre-exponential factor using the Kissinger variable heating rate iso-conversion method (, ) and activation energy and reaction order by the Farjas method ( for thermally unstable materials. The test method is applicable to the temperature range from 300 to 900 K (27 to 627°C). )
1.2 Both nth order and accelerating reactions are addressed by this method over the range of 0.5 < n < 4 and 1 < p < 4 where n is the nth order reaction order and p is the Avrami reaction order (. Reaction orders )n and p are determined by the Farjas method (. )
1.3 This test method uses the same experimental conditions as Test Method . The Flynn/Wall/Ozawa data treatment of Test Method may be simultaneously applied to these experimental results.
1.4 The values stated in SI units are to be regarded as standard. No other units of measurement are included in this standard.
1.5 There is no ISO equivalent to this standard.
1.6 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety, health, and environmental practices and determine the applicability of regulatory limitations prior to use.
1.7 This international standard was developed in accordance with internationally recognized principles on standardization established in the Decision on Principles for the Development of International Standards, Guides and Recommendations issued by the World Trade Organization Technical Barriers to Trade (TBT) Committee.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
E473 Terminology Relating to Thermal Analysis and Rheology
E537 Test Method for The Thermal Stability of Chemicals by Differential Scanning Calorimetry
E691 Practice for Conducting an Interlaboratory Study to Determine the Precision of a Test Method
E698 Test Method for Kinetic Parameters for Thermally Unstable Materials Using Differential Scanning Calorimetry and the Flynn/Wall/Ozawa Method
E967 Test Method for Temperature Calibration of Differential Scanning Calorimeters and Differential Thermal Analyzers
E968 Practice for Heat Flow Calibration of Differential Scanning Calorimeters
E1142 Terminology Relating to Thermophysical Properties
E1231 Practice for Calculation of Hazard Potential Figures of Merit for Thermally Unstable Materials
E1860 Test Method for Elapsed Time Calibration of Thermal Analyzers
E1970 Practice for Statistical Treatment of Thermoanalytical Data
E2041 Test Method for Estimating Kinetic Parameters by Differential Scanning Calorimeter Using the Borchardt and Daniels Method
E2161 Terminology Relating to Performance Validation in Thermal Analysis and Rheology
ICS Number Code 17.200.10 (Heat. Calorimetry)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM E2890-12(2018), Standard Test Method for Kinetic Parameters for Thermally Unstable Materials by Differential Scanning Calorimetry Using the Kissinger Method, ASTM International, West Conshohocken, PA, 2018, www.astm.orgBack to Top